MAGNETIC STRUCTURES. 2.1 Meanfield theory of magnetic ordering


 Egbert Watkins
 1 years ago
 Views:
Transcription
1 2 MAGNETIC STRUCTURES The meanfield theory introduced in the previous section is used in this chapter as a basis for examining some of the magnetic structures assumed by the rare earth metals. The theory is presented at length in the first section. Beginning with the expression for the free energy, some general results are established for the magnetization, and applied analytically to the calculation of the susceptibility in the hightemperature limit. The meanfield approximation is then developed, and a numerical method for solving the resulting equations selfconsistently, for magnetic structures which are commensurable with the lattice, is described. The Landau expansion of the free energy in terms of the order parameters of the magnetic system provides the starting point for a discussion of a number of the periodic magnetic structures which arise as a result of the long range of the indirectexchange interaction. The ordering temperatures are calculated by analytical means, and the relative stability of different structures compared. In the following section, the important extension by Callen and Callen of the Zener powerlaw for the temperature dependence of the magnetic anisotropy is derived. The thermal expectation values Ol m of the Stevens operators are calculated and their dependence on the magnetization determined. From the free energy, the magnetic anisotropy and the magnetoelastic coefficients are deduced. We conclude with a detailed discussion of some magnetic structures, using the aforementioned analytical methods, supplemented by numerical calculations, to help identify those characteristics of the magnetic interactions which lead to the stability of different momentconfigurations under various conditions. This account is illustrated by various examples, with emphasis on the the diverse magnetic phases of Ho. Among other structures, we consider the ferromagnet, thecone, the helix, thelongitudinal wave, thecycloid, and commensurable spin slips. The effect of a magnetic field in stabilizing fan and helifan structures, and the ordering of thin films and superlattices, are also discussed. 2.1 Meanfield theory of magnetic ordering The simplest form of Hamiltonian which is adequate to explain the occurrence of most of the observed magnetic structures is H = H cf (i) 1 J (ij) J i J j + H 2 Z, (2.1.1a) i ij
2 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 69 where the first sum is the singleion crystalfield Hamiltonian H cf (i) = Bl 0 Ol 0 (J i )+B6O 6 6(J 6 i ), l=2,4,6 (2.1.1b) the twoion term is assumed to be isotropic, and the Zeeman term is H Z = i µ i H i. (2.1.1c) The field may vary spatially, so that we must specify its value on each site, writing H i H(R i ), and the magnetic moment on the ith ion is µ i = gµ B J i. The staticsusceptibility tensor may be derived as the second derivative of the free energy, and we shall therefore begin by recapitulating a few basic thermodynamic results. The free energy is F = U TS = 1 ln Z, (2.1.2) β where U is the internal energy, S the entropy, and β =(k B T ) 1. The partition function is Z =Tr { e βh} = p e βe p. (2.1.3) Tr indicates the trace over a complete set of states, and the final summation may be performed if the eigenvalues E p of the Hamiltonian are known. The expectation value of an operator A is A = 1 Z Tr{ Ae βh}. (2.1.4) The derivative of the free energy with respect to a variable x is F x = 1 Z βz x = 1 { } H Z Tr x e βh = H. (2.1.5) x This expression is obtained by utilizing the invariance of the trace to the basis used, assuming it to be independent of x and a cyclic permutation of the operators, thus allowing a conventional differentiation of the exponential operator, as may be seen by a Taylor expansion. This result is general, but the exponential operator can only be treated in this simple way in second derivatives if H/ x commutes with the Hamiltonian, which is usually not the case. However, we may be interested only in the leadingorder contributions in the limit where β is small, i.e. at high
3 70 2. MAGNETIC STRUCTURES temperatures. Expanding in powers of β, we may use the approximation exp{ βh} 1 βh β2 H 2. In this case, we may proceed as above, and the result is 2 F x y = 2 H ( H H H + β x y x y x β2 [ H 2 x, H y H ) y ] H + O(β 3 ), (2.1.6) where the second and higherorder terms vanish if one of the derivatives of H commutes with H itself. In many instances, it is more convenient to consider the angular momentum rather than the magnetic moment, with a corresponding field variable h i = gµ B H i, so that the Zeeman term (2.1.1c) becomes H Z = i µ i H i = i J i h i. (2.1.7) Since the exchange and anisotropy terms in H do not depend explicitly on the field, H/ H iα = µ iα and, using eqn (2.1.5), we have µ iα = F/ H iα or J iα = F/ h iα. (2.1.8) Next, we define the nonlocal susceptibilities χ µ αβ (ij) = µ i / H jβ = 2 F/ H iα H jβ, (2.1.9a) and similarly χ J αβ (ij) =(gµ B ) 2 χ µ αβ (ij) = 2 F/ h iα h jβ, (2.1.9b) and the corresponding Fourier transforms, e.g. χ J αβ(q) = 1 χ J N αβ(ij)e iq (Ri Rj) = χ J αβ(ij)e iq (Ri Rj). ij j (2.1.9c) The final equality only applies in a uniform system. If the field is increased by an infinitesimal amount δh(q)exp(iq R i ), the individual moments are changed by δ µ iα = χ µ αβ (ij)δh β(q)e iq Rj, (2.1.10a) j β according to (2.1.9). Hence the added harmonicallyvarying field introduces one Fourier component in the magnetization: δm α (q) = 1 δ µ V iα e iq Ri = N χ µ V αβ (q)δh β (q), (2.1.10b) i β
4 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 71 proportional to the susceptibility at the wavevector considered. The usual definition of the susceptibility components (per unit volume), as used in Chapter 1, is δm α (q)/δh β (q). The susceptibility used in (2.1.10b)differsfromthisbythefactorV/N, i.e. we are here considering the susceptibility per atom instead of per unit volume. Furthermore, since we shall not make any further use of χ µ αβ (q), we shall reserve the notation χ αβ (q) fortheqdependent susceptibility χ J αβ (q), introduced in eqn (2.1.9b), throughout the rest of the book. So in terms of the susceptibility per atom, in units of (gµ B ) 2, the above equation may be written δ J α (q) = 1 δ J iα e iq Ri = χ N αβ (q)δh β (q), (2.1.10c) i β with the upper index J in χ J αβ (q) being suppressed from now on The hightemperature susceptibility In order to calculate χ(q) in zero field, we shall first use the approximation (2.1.6) to the derivative of the free energy, valid at high temperatures. In this limit J i = 0, and only one term in the expansion is nonzero: χ αβ (ij) =βtr { J iα J jβ (1 βh) }/ Tr { 1 βh }, (2.1.11) to second order in β. The commutator in the third term on the righthand side of (2.1.6) is either zero or purely imaginary (if i = j and α β), showing immediately that the expectation value of this term must vanish in all cases. To first order in β, we obtain from (2.1.11) χ αβ (ij) βtr { J iα J jβ }/ Tr { 1 } = 1 3 J(J +1)βδ αβ δ ij, using the product of the eigenvectors of J iα as the basis, and recalling that m 2 = 1 3J(J + 1)(2J +1), when m runs from J to J. In order to calculate the secondorder contribution, we shall utilize the general tensor properties of the Stevens operators, which satisfy the orthogonality condition: Tr { Ol m (J i )Ol m (J j) } = δ ij δ ll δ mm Tr { [Ol m (J i )] 2} and Tr { Ol m (J i ) } =0, (2.1.12) when l and l are both nonzero. O 0 0 is just the identity operator. J iα is a linear combination of O m 1 (J i), m = 1, 0, 1, and (2.1.12) then implies
5 72 2. MAGNETIC STRUCTURES that the trace of the Hamiltonian (2.1.1) vanishes, and hence that the denominator in (2.1.11) is Tr{1} =(2J +1) N. For the secondorder term in the numerator, we find Tr { J iα J jβ H } = δ ij B2 0 Tr { J iα J iβ O2(J 0 i ) } J(ij)Tr { } J iα J jβ J i J j = δ ij δ αβ B 0 2 Tr{ J 2 iα [3J 2 iz J(J +1)]} δ αβ J (ij)tr { J 2 iα J 2 jα}, utilizing that J iα J jβ is a linear combination of second and lowerrank tensors for i = j, and a product of firstrank tensors for i j. When α = z (or ζ), we may readily calculate the first trace, using m 4 = 1 15 J(J + 1)(2J + 1)(3J 2 +3J 1). The traces with α = x or α = y must be equal, and using this equality in the case α = x, for instance, we may replace Jx 2 in the trace by 1 2 (J x 2 + Jy 2 ) 1 2 J(J +1) 1 2 J z 2. As the constant term multiplied by 3Jz 2 J(J + 1) does not contribute (as Tr{3J z 2 J(J +1)} = 0), the trace with α = x or y is equal to 1/2 times that with α = z. Only the singleion terms contribute to the trace when i = j (J (ii) is assumed to be zero), and of these only the lowestrank term B2 0 appears, to leading order. The twoion coupling only occurs in the trace, and hence in χ αβ (ij), when i j, and this contribution may be straightforwardly calculated. To second order in β, the offdiagonal terms are zero, whereas 1 χ αα (ij) =δ ij 3 J(J +1)β[ (3δ αζ 1)B2(J )(J )β] + [ 1 3 J(J +1)β] 2 J (ij). Introducing the Fourier transform of the twoion coupling, J (q) = j J (ij)e iq (Ri Rj), (2.1.13) we find that, to the order considered, the inverse of the qdependent susceptibility may be written 1/χ αα (q) = 3k B T J(J +1) +(3δ αζ 1)6(J 1 2 )(J ) B2 0 J(q)+O(1/T ). 5J(J +1) (2.1.14) The inverse susceptibility in the hightemperature limit thus increases linearly with the temperature, with a slope inversely proportional to the square of the effective paramagnetic moment ( {J(J +1)} 1/2 ). The susceptibilities determined experimentally by magnetization measure
6 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 73 Fig The inverse susceptibility, in atomic units, in Tm above T N. The full lines depict the results of a meanfield calculation and the dashed lines are extrapolations of the hightemperature limit. Experimental values are also shown. The MF theory predicts a deviation from the hightemperature expression as the ordering temperature is approached from above, because of crystalfield anisotropy effects. ments are the bulk values at zero wavevector. The straight lines found at high temperatures for the inversesusceptibility components 1/χ αα (0) versus temperature may be extrapolated to lower values, as illustrated in Fig The values at which these lines cross the temperature axis are the paramagnetic Curie temperatures θ and θ, determined respectively when the field is parallel and perpendicular to the caxis (ζaxis). The hightemperature expansion then predicts these temperatures to be k B θ = 1 3 J(J +1)J (0) 4 5 (J 1 2 )(J )B0 2, (2.1.15a) and k B θ = 1 3 J(J +1)J (0)+ 2 5 (J 1 2 )(J )B0 2. (2.1.15b) Hence the paramagnetic Curie temperatures are determined by the lowestrank interactions in the Hamiltonian, i.e. those terms for which l +l = 2. The difference between the two temperatures depends only on B2 0, because of the assumption that the twoion coupling is an isotropic
7 74 2. MAGNETIC STRUCTURES Heisenberg exchange. The mean temperature (θ +2θ )/3 is determined by J (0) which, from (2.1.13), is the algebraic sum of the isotropic twoion interactions, and this temperature may be measured directly with a polycrystalline sample. The two basalplane components are found to be equal. This is not just due to the assumption of high temperatures, but is generally valid as long as there is no ordered moment in the basalplane. In this case, the caxis is a threefold symmetry axis, or effectively a sixfold axis, due to the symmetry of the basalplane anisotropy B 6 6 in the Hamiltonian. The susceptibility is a secondrank tensor, according to (2.1.9), and it cannot therefore vary under rotation about a three or sixfold axis The meanfield approximation The hightemperature expansion may be extended to higher order in β, but the calculations rapidly become more complex, so we shall instead adopt another approach, the meanfield approximation. In this method, the correlated fluctuations of the moments around their equilibrium values are neglected. In order to introduce J i into the Hamiltonian, we utilize the identity J i J j =(J i J i ) (J j J j )+J i J j + J j J i J i J j. The MF approximation then consists in neglecting the first term on the righthand side, which is associated with twosite fluctuations, since i j. The Hamiltonian (2.1.1) is then effectively decoupled into a sum of N independent terms for the single sites; H i H MF (i), where H MF (i) =H cf (i) J i h i ( J i 1 2 J i ) J (ij) J j, (2.1.16) in the presence of an external magnetic field h i = gµ B H i. Introducing the effective field h eff i = h i + J (ij) J j, (2.1.17a) j we may write the MF Hamiltonian H MF (i) =H cf (i) J i h eff i j J i (h eff i h i ). (2.1.17b) Selfconsistent solutions of the MF equations may sometimes be obtained analytically, but numerical methods may be used more generally, provided that the periodicity of the magnetic structure is commensurable with that of the lattice. For an assumed distribution of J j, the effective field and hence the MF Hamiltonian for the ith site is calculated.
8 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 75 Diagonalizing this Hamiltonian, we may derive the partition function Z i, the free energy F i, and the expectation value J i for this site. The last term in (2.1.17b) just adds a constant contribution to F i, without affecting J i. Performing this calculation for all the different ions, we determine the various values of J j, and the total free energy is the sum of the F i. The derived values of J j are used as the input for a new MF Hamiltonian, and this iterative procedure is repeated until selfconsistency is attained. The selfconsistent solution of the MF Hamiltonian may be one in which J i is nonzero even in zero field, thus describing the occurrence of a spontaneous ordering of the moments. Having found the selfconsistent solution for the angular momenta, we may proceed to calculate the susceptibility. The MF Hamiltonian for the ith site has been diagonalized, and we shall denote the (2J +1) eigenstates by p>, with corresponding energy eigenvalues E p. If the effective field is changed by a small amount δh eff β, the Zeeman term J iβδh eff β must be added to the Hamiltonian, and E (1) p = E p <p J iβ p>δh eff β, to first order in the perturbation, provided that p> is a set which diagonalizes the perturbation within the possibly degenerate subspaces of the zerofield Hamiltonian. The new eigenstates are p (1) > = p> δh eff β p >< p J iβ p>/(e p E p ), p where the terms for which E p = E p vanish. Using (2.1.3) and (2.1.4), we then have, to first order in δh eff β, J (1) iα = p <p (1) J iα p (1) >n (1) p δh eff β δh eff β = p <p Jiα p >< p J iβ p>n p /(E p E p ) pp <p J iα p>n (1) p <p Jiβ p >< p J iα p>n p /(E p E p ), pp where the last two sums extend over states for which E p E p. The population factor of the pth level at δh eff β =0isn p =exp( βe p )/Z i, and n (1) p we find is the corresponding factor at the field δh eff β. By differentiation, n (1) p / (δheff β )={ <p J iβ p> <p J iβ p >n p } βnp p = { <p J iβ p> J iβ } βn p. Introducing this result in the equation above, and interchanging p and
9 76 2. MAGNETIC STRUCTURES p in the last sum, we obtain finally: χ o αβ (i) = J iα / heff β + β E p =E p Ep Ep = <p J iα p >< p J iβ p> (n E p pp E p n p ) p pp <p J iα p >< p J iβ p>n p β J iα J iβ. (2.1.18) The second summation is transformed in such a way that it is no longer necessary for J iβ to be diagonal within the degenerate subspaces, as required initially. The first term in the susceptibility is the Van Vleck contribution, which becomes constant at zero temperature, whereas the second term, the Curie contribution, diverges as 1/T in the lowtemperature limit. The susceptibility deduced above is that determining the response,whereaswewish to know the response due to a small change of the external field. If a small harmonicallyvarying field δh q exp(iq R i ) is applied, the effective field, according to (2.1.17a), is due to a change of the effective field, δ J i = χ o (i)δh eff i δh eff i = δh q e iq Ri + j J (ij)χ o (j)δh eff j. This equation may be solved by a Fourier transformation if χ o (i) =χ o is siteindependent, which it is so long as J i is independent of i, as in the hightemperature paramagnetic phase, for example, where J i = 0. Neglecting any sitedependence of χ o, and introducing the notation δh eff i = δh eff q exp(iq r i ), we get δh eff q = { 1 χ o J (q) } 1 δhq, or, by the definition of the susceptibility, χ(q) = { 1 χ o J (q) } 1 χ o. (2.1.19a) In the following, we shall assume that the external magnetic field is zero. With this restriction, χ(q) is diagonal in the (ξηζ)coordinate system, and the reciprocal susceptibility, in the MF approximation, may be written 1/χ αα (q) =1/χαα o J(q). (2.1.19b) In the degenerate case, (2.1.18) implies that χαα o = βj(j +1)/3. However, if H cf is nonzero, the expression (2.1.18) for the susceptibility becomes quite complex. A drastic simplification is achieved by assuming a
10 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 77 small value of β. In this high temperature limit, χ o may be calculated by a procedure equivalent to that used in deriving (2.1.14), except that J (ij) = 0. Hence, to second order in β, wehave χ o αα 1 3 J(J +1)β[ (3δ αζ 1)(J 1 2 )(J )B0 2β ]. (2.1.20) Introducing (2.1.20) in (2.1.19), we obtain the same result as previously derived in (2.1.14), demonstrating that the MF approximation is correct in the hightemperature limit. Although the thermal fluctuations increase when the temperature is raised, they also become increasingly uncorrelated. It is the latter effect which is the most pronounced, and the correction to the MF value of the free energy, proportional to the correlation energy of the twosite fluctuations J (ij){ J i J j J i J j }, decreases with temperature at high temperatures. In the other limit of zero temperature, the correlation effects are much stronger, but the fluctuations themselves are small. We may therefore also expect the MF approximation to be accurate in this limit, and to provide a useful interpolation at intermediate temperatures. χ o increases steadily with decreasing temperature. If the crystalfield ground state is degenerate, the second sum in (2.1.18) is nonzero and χ o diverges in the zerotemperature limit. Because of the Kramers degeneracy, the ground state is always at least doubly degenerate if 2J is odd. When J is an integer, the ground state may be a singlet, in which case χ o saturates at a constant value at zero temperature. Except in this special case, it is always possible to find a temperature where 1/χ αα (q) is zero, corresponding to an infinite χ αα (q). The largest value of the qdependent susceptibility is found at the wavevector Q at which J (q) has its maximum. Of the three nonzero components of χ(q), the cccomponent is the largest if B2 0 is negative. If B2 0 is positive, on the other hand, the two equal basalplane components are the largest. It is the maximum component of the susceptibility at q = Q which first diverges when the system is cooled. This divergence signals that the paramagnetic groundstate becomes unstable against the formation of an ordered state in which the moments are modulated with the wavevector Q, and point along or perpendicular to the cdirection, depending on whether B2 0 is respectively negative or positive. Hence, a secondorder phase transition takes place at this critical temperature, called the Curie temperature, T C,ortheNéel temperature, T N, depending on whether Q = 0 or Q 0. JustbelowT N, the ordered moment J i is small, and thefreeenergyoftheith ion may be expanded in powers of this moment. In order to establish this expansion, we first consider the Hamiltonian H (i) =H cf (i) J i h. The corresponding free energy may be written F i = F 0 /N J i h + α A α J iα 2 + αβ B αβ J iα 2 J iβ 2 +.
11 78 2. MAGNETIC STRUCTURES Except for the field term, this expansion only includes products of components in which the sum of the exponents is even, because of timereversal symmetry. Using the equilibrium condition F i / J iα =0, and recalling that J iα = χαα(σ o =0)h α to leading order, in the zerofield limit, we obtain A α = { 2χ o αα(σ =0) } 1, (2.1.21a) where χαα o (σ = 0) is the MF susceptibility (2.1.18), in the limit of zero magnetization (field). The susceptibility decreases with increasing magnetization (or field), as described by the fourthorder terms. An orderofmagnitude estimate of B αβ may be obtained by neglecting H cf (i). In this case, the magnetization as a function of the field is given by the Brillouin function (1.2.31): J iα = JB J (βjh α ) 1 3 J(J +1)βh { α (J 2 + J )β2 h 2 α}, which, in combination with the equilibrium condition for the free energy, determines B αα. The offdiagonal terms may be obtained straightforwardly by utilizing the condition that, when H cf (i) is neglected, the free energy should be invariant with respect to any rotation of the magnetization vector, implying that all the coefficients B αβ are equal, or B αβ 9 J 2 + J J 3 (J +1) 3 k B T. (2.1.21b) The introduction of the crystalfield terms of course modifies this result, but rather little in the hightemperature limit. Under all circumstances, the effective sixfold symmetry around the caxis implies that B αβ is symmetric, B ξξ = B ηη = B ξη,andb ξζ = B ηζ, and it also eliminates the possibility that any other fourthorder terms may contribute. The expansion of the free energy of the total system, when the external field is zero, is obtained from the expansion of F i, summed over i, by substituting the exchange field h eff i = j J (ij) J j for h, and adding the constant 1 2 J i h eff i,sothat F = F 0 1 J (ij) J i J j + [ A 2 α J iα 2 + B αβ J iα 2 J iβ 2] ij i α αβ (2.1.22) to fourth order in the magnetization. This expansion of the free energy in terms of the order parameter(s) is called the Landau expansion. Assuming the ordered phase to be described by a single wavevector, we may write J iα = Jσ α cos(q R i + ϕ α ), (2.1.23)
12 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 79 where σ α = σ α (q) is the relative magnetization at the wavevector q. Introducing this into the freeenergy expression, and utilizing the condition that i cos(q R i + ϕ) =0,ifq is not a reciprocal lattice vector, we find f =(F F 0 )/N = 1 4 J 2 α {2A α J(q)}σ 2 α J 4 αβ B αβ {2+cos2(ϕ α ϕ β )}σ 2 ασ 2 β, (2.1.24) if 4q is different from a reciprocal lattice vector. The coefficients of the second power are thus {2A α J(q)} =1/χ αα (q,σ =0),where the susceptibility is evaluated at zero magnetization. As long as all the secondorder coefficients are positive, at any value of q, the free energy is at its minimum when σ α = 0, i.e. the system is paramagnetic. The smallest of these coefficients are those at q = Q, wherej (q) hasits maximum. In the heavy rare earths, with the exception of Gd, Q is nonzero and is directed along the caxis. Depending on the sign of B2, 0 the magnetic structures occurring in the heavy rare earths may be divided into two classes, which we will discuss in turn Transversely ordered phases When B2 0 > 0, as in Tb, Dy, and Ho, the two basalplane components of χ(q) both diverge at the same critical temperature T N. Using the approximate hightemperature value (2.1.20) for the susceptibility, we find that 1/χ ξξ (Q,σ =0)=1/χ ηη (Q, 0) = 2A ξ J(Q) vanishes at the temperature determined by k B T N 1 3 J(J +1)J (Q)[ (J 1 2 )(J )B0 2/k B T N ]. (2.1.25) Below T N,bothσ ξ and σ η are generally nonzero at the wavevector Q, and the free energy f, given by (2.1.24) with σ ζ = 0, is minimized when σ ξ (Q) =σ η (Q) =σ Q,and ( ) 1/2 J (Q) 2Aξ σ Q = 4J 2 ; ϕ B ξ ϕ η = ± π ξξ 2, (2.1.26a) corresponding to the helical ordering: J iξ = Jσ Q cos (Q R i + ϕ) J iη = ±Jσ Q sin (Q R i + ϕ). (2.1.26b) The length of the angularmomentum vector is Jσ Q, independent of the site considered. There are two energeticallydegenerate configurations,
13 80 2. MAGNETIC STRUCTURES a right or a lefthanded screw, depending on the choice of sign. From the condition 1/χ ξξ (Q, 0) (T T N ), sufficiently close to T N,weget the usual MF result that the order parameter σ Q (T N T ) 1/2. Although 1/χ ξξ (Q, 0) becomes negative below T N, the inverse of the actual susceptibility, 1/χ ξξ (Q) =1/χ ξξ (Q,σ Q ), does not. Analogously to the derivation of A α in (2.1.21a), it may be seen that 1/χ ξξ (Q) is a second derivative of the free energy, i.e. 1/χ ξξ (Q) = 2 f/ (Jσ Q ) 2 1/χ ξξ (Q,σ =0)+12J 2 B ξξ σ 2 Q = 2/χ ξξ (Q,σ =0). Hence, 1/χ ξξ (Q) is nonnegative, as it must be to ensure that the system is stable, as is also the case for any other component of the susceptibility. Because J i is constant, the umklapp contributions to the free energy in (2.1.24), for which 4Q is a multiple of the reciprocallattice parameter 4π/c, cancel. The free energy of the helix is therefore independent of the lattice, at least to the fourth power in the magnetization. If the anisotropy terms in H cf can be neglected, the helix is the most stable configuration satisfying the condition that J i = Jσ is constant. With this constraint, only the twoion interaction term in the free energy (2.1.22) may vary, and this may be minimized by the method of Lagrange multipliers (Nagamiya 1967). We will begin with the weaker constraint; i J i 2 = N(Jσ) 2 is constant, which means that we have to minimize the energy expression U = 1 J (ij) J i J j + λ ( Ji 2 (Jσ) 2) 2 ij i = N { (2.1.27a) 1 2 J (q)+λ} J(q) J( q) Nλ(Jσ) 2, q where the introduction of J i = q J(q) exp(iq R i), as in (2.1.10c), yields the second form. Minimizing this expression with respect to J( q), we obtain the following equation: U/ J( q) = N { J(q)+2λ } J(q) =0, assuming J ( q) =J (q). For a given value of λ, this condition is only satisfied if either J(q) = 0, orifq = q λ,wherej (q λ )=2λ, which implies that only J(q λ ) may be nonzero. Introducing this condition in U, we find U = Nλ(Jσ) 2 = 1 2 NJ (q λ )(Jσ)2, (2.1.27b)
14 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 81 which is then minimized with respect to q when q λ = Q, at which wavevector J (q) has its maximum. Hence the twoion energy attains its minimum when only the two Fourier components J i (±Q) are nonzero. The stronger constraint that J i should be constant is then met only by the helix (2.1.26). In the zerotemperature limit, this constraint derives from the fact that the moments attain their saturation value, J i = J, immediately the exchange field is not identically zero, since χαα(σ o =0) diverges in this limit when H cf = 0. At elevated temperatures, it is clear that the sum of the singleion terms in the free energy (the A and Bterms in (2.1.22)) is most effectively minimized if the minimum condition is the same for all the ions. When H cf =0,thereareno restrictions on the plane in which the moments spiral; it may be rotated freely, without change in energy, as long as J i is constant and all the components vary with the wavevector Q. This behaviour is analogous to that of the Heisenberg ferromagnet, which may be considered as a helically ordered system with Q = 0. If Q is not perpendicular to the plane in which the moments lie, the structure is called the tilted helix (Elliott 1971; Sherrington 1972) and the extreme case, with Q in the plane of the moments, is the cycloidal structure. When B2 0 > 0, the orientation of the plane is stabilized to be perpendicular to the caxis, and with Q along this axis we obtain the true helical structure. If B2 0 > 0 is the only crystalfield parameter of importance, the regular helix is the stable structure in the whole temperature interval between zero and T N. If the Landau expansion (2.1.22) is continued to the sixth power in the magnetization, a term appears proportional to B6 6, distinguishing between the a andbdirections in the basalplane. Instead of using this expansion, we shall consider the alternative expression for the free energy, to leading order in B6, 6 F F 1 1 J (ij) J i J j + B6 6 2 O6 6 (J i) ij i = F 1 1 (Jσ) 2 J (ij)cos(φ 2 i φ j )+ (2.1.28) κ 6 6 cos 6φ i, ij i where J i = Jσ(cos φ i, sin φ i, 0) and F 1 is the part independent of φ i. The expectation values are those obtained in the limit B6 6 = 0, i.e. σ and κ 6 6 are assumed to be independent of the angle φ i. The presence of the sixfold anisotropy term distorts the helix. In order to solve the equilibrium equation F/ φ i =(Jσ) 2 J (ij)sin(φ i φ j ) 6κ 6 6 sin 6φ i =0, j we introduce the expansion φ i = u i + γ sin 6u i + ; u i = Q R i, (2.1.29a)
15 82 2. MAGNETIC STRUCTURES using the series exp[i(u + γ sin 6u)] = J 0 (γ)e iu + J 1 (γ) ( e i7u e i5u) + J 2 (γ) ( e i13u + e i11u) + e iu + γ 2 ( e i7u e i5u), (2.1.29b) where J n (x) are the Bessel functions. To leading order in γ, the equilibrium equation then gives γ = 12κ 6 6 (Jσ) 2{ 2J (Q) J(5Q) J(7Q) }, (2.1.30a) and the free energy is reduced proportionally to γ 2 : F/N = F 1 /N 1 2 (Jσ)2 J (Q) 1 8 (Jσ)2{ 2J (Q) J(5Q) J(7Q) } γ 2. (2.1.30b) The hexagonal anisotropy introduces harmonics, of equal magnitude, in the basalplane moments at the wavevectors 6Q ± Q and, in higher order, at the wavevectors 6mQ±Q. Ifκ 6 6, and thus also γ, are negative, the easy directions in the plane are the aaxes. In the special case where the angle u i = π/12, i.e. the unperturbed ith moment is halfway between an easy and a hard direction, the largest change φ i u i = γ occurs in the orientation of the moments, and the angle to the nearest easy direction is reduced, since u i lies between 0 and π/6, and κ 6 6 is negative. The moments in the helix are therefore distorted so that they bunch around the easy axes. The above calculation is not valid if Q is 0 or 2π/c, when the hexagonal anisotropy may be minimized without increasing the exchange energy, as it may also if the (average) turn angle ω of the moments from one hexagonal plane to the next is a multiple of 60,sothat6Q is an integer times 4π/c. The products of the fifth and seventh harmonics introduce additional umklapp contributions to the free energy if 12Q is a multiple of the effective reciprocallattice spacing 4π/c, implying that the cases where ω is p30 and p =1, 3, 5 are also special. In higher order, corrections appear whenever m12q = p4π/c, wherem and p are integers and 0 p 6m, i.e. at any commensurable value of Q, but the corrections decrease rapidly with m, excluding cases where m and p have common factors. In contrast to the result found above, the commensurable contributions depend on the absolute phase ϕ in (2.1.26b), and an adjustment of this phase will quite generally allow the system to reduce the anisotropy energy through the umklapp terms. This change in energy may compensate for the increase in the exchange energy when the ordering wavevector Q is changed from its value Q = Q 0,atwhich
16 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 83 J (q) has its maximum, to a nearby commensurable value Q c. Hence the hexagonal anisotropy couples the helical magnetic structure to the lattice, and it may induce continuous or abrupt changes of the ordering wavevector as a function of temperature, as discussed, for instance, by Bak (1982). In Ho, 12Q 0 is close to 4π/c, and the hexagonal anisotropy is large at low temperatures. Experimental investigations have shown that a number of commensurable values of Q are stabilized in this system, as we shall discuss in more detail in the last section of this chapter Longitudinally ordered phases When B 0 2 is negative, as in Er and Tm, χ ζζ (Q) is the component of the susceptibility which diverges at the highest temperature, and the hightemperature expansion predicts that 2A ζ J(Q) vanishes at a critical temperature determined by k B T N 1 3 J(J +1)J (Q)[ (J 1 2 )(J )B0 2 /k B T N]. (2.1.31) Just below this temperature, only the component σ ζ at the wavevector Q is nonzero and, from the free energy expansion (2.1.24), f/ σ ζ =0 determines the relative magnetization as ( ) 1/2 J (Q) 2Aζ σ ζ (Q) =σ Q = 3J 2. (2.1.32) B ζζ The free energy is independent of the phase ϕ = ϕ ζ,sowesetϕ =0. If we add another Fourier component with q ±Q: J iζ = Jσ Q cos (Q R i )+Jσ q cos (q R i + ϕ ) (2.1.33) then, if mq ± nq is different from a reciprocal lattice vector, where m and n are integers and m + n = ±4, the free energy is f = 1 4 J 2[ {2A ζ J(Q)}σQ 2 + {2A ζ J(q)}σq 2 ] J 4 [ B ζζ 3σ 4 Q +3σq 4 +12σQ 2 σ2 q +4σ3 Q σ q δ q,±3q cos ϕ +4σ Q σq 3 δ 3q,±Q cos 3ϕ ]. (2.1.34) This result shows that, if q =3Q or q = 1 3Q, there is an extra fourthorder contribution to the free energy (q q represents the same structure with ϕ ϕ ). Of these two special cases, the one where q =3Q is the most interesting, because the extra term is linear in σ 3Q. This means that the third harmonic appears simultaneously with the basic Fourier component at Q. Minimizing the free energy given by (2.1.34), we find σ 3Q = J 2 B ζζ J (Q) J(3Q) σ3 Q ; ϕ = ϕ + π, (2.1.35a)
17 84 2. MAGNETIC STRUCTURES neglecting a term proportional to σq 2 in the denominator. The 3Qcomponent is thus proportional to σq 3, and hence to (T N T )3/2. Denoting the wavevector at which J (q) has its maximum by Q 0,weconclude that the appearance of the third harmonic implies that f has its minimum at a value of Q slightly different from Q 0. Minimizing the free energy with respect to Q along the caxis, by requiring f/ Q =0,we obtain to leading order Q = Q 0 3 J (3Q 0 ) J (Q 0 ) ( σ3q σ Q ) 2. (2.1.35b) J (Q 0 ) is negative, so the shift Q Q 0 has the same sign as J (3Q 0 ) and is proportional to (T N T ) 2. The other special case, 3q = Q, reflects the possibility that, if J (Q 0 /3) is close to J (Q 0 ), the system may reduce its energy by making a first order transition to a state where Q Q 0 /3 is the fundamental wavevector, with the third harmonic being close to Q 0. The presence of a term in the free energy cubic in the order parameter, σ Q/3 in this case, implies that the transition becomes of first order, so that the order parameter changes discontinuously from zero to a finite value. The Q 0 /3transition appears to be of no importance in real systems, so we shall return to the discussion of the other case. If the free energy is expanded to higher (even) powers in the relative magnetization, it is clear that the (2n + 2)power term leads to a contribution proportional to σ (2n+1)Q σ 2n+1 Q which, in combination with the term quadratic in σ (2n+1)Q, implies that the ordering at the fundamental wavevector Q induces a (2n + 1)harmonic proportional to σ 2n+1 Q (T N T ) (2n+1)/2. Starting as a pure sinusoidally modulated wave at T N, the moments approach the square wave J iζ = 4J ( cos x 1 π 3 cos 3x cos 5x 1 7 cos 7x + )x=q R, i+ϕ (2.1.36a) in the limit of zero temperature where J iζ = ±J, neglecting strong anisotropy effects. Although the behaviour of the angular momentum is simple, the dependence of the free energy on the wavevector is complicated. It is only when the ordering is incommensurable, i.e. mq is different from any multiple of the length 4π/c of the reciprocallattice vector along the caxis, that the energy of the squarewave structure at T =0is f(0) = H cf 4J 2 π 2 { J (Q)+ 1 9 J (3Q) J (5Q)+ }. (2.1.36b) An infinitesimal change of the ordering wavevector from Q, which minimizes f(0), to Q c may make it commensurable with the lattice, so that
18 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 85 mq c = p(4π/c) and additional umklapp terms contribute to the free energy. Again these contributions depend on the absolute phase ϕ, and there will always be values of Q c close to Q leading to a lower free energy than that obtained in the incommensurable case. In the lowtemperature limit, the modulation of the caxis moment is therefore locked to the lattice periodicity. This tendency is already apparent close to T N. In the expansion of the free energy considered above for m =4,umklapp terms modify the fourthpower coefficient, and analogous effects occur in higher powers of the magnetization. This indicates that the system may stay commensurable even near T N although, in the close neighbourhood of T N, the critical fluctuations neglected here may oppose this tendency. The optimal value of Q c may change as a function of temperature, in which case the system will exhibit a number of firstorder, or possibly continuous, transitions from one commensurable structure to another. Of these structures, those for which Q c =3Q c =5Q c =, i.e. Q c =0 or 2π/c, are particularly stable, as they only involve one wavevector, so that f(0) = H cf 1 2 J 2 J (Q c ) (in this connection, we note that = π2 /8). The anisotropic Isingmodel with competing interactions, the socalled ANNNI model, is a simplified version of the above, and it shows a rich variety of different incommensurable, commensurable, and chaotic ordered structures as a function of temperature and the coupling parameters (Bak 1982) Competing interactions and structures The complex behaviour of the longitudinally ordered phase is a consequence of the competition between the singleion part of the free energy, which favours a structure in which the magnitude of the moments varies as little as possible, particularly at low temperature, and the twoion contributions, which prefer a singleq ordering. When B2 0 is positive, helical ordering satisfies both tendencies without conflict. This points to another alternative which the longitudinal system may choose. Although χ ζζ (Q) decreases below T N, the two perpendicular components continue to increase, and they may therefore diverge at a lower temperature T N. Assuming the expansion (2.1.24) of the free energy still to be valid at T N, and neglecting the third and higher harmonics of J iζ, we may write it: f = f(σ Q )+ 1 4 J 2 α=ξ,η [ 2Aξ J(Q)+B ξζ (Jσ Q ) 2 {2+cos2(ϕ α ϕ)} ] σ 2 α J 4 B ξξ [ 3σ 4 ξ +3σ 4 η +2{2+cos2(ϕ ξ ϕ η )}σ2 ξ σ2 η]. (2.1.37) The effective coefficient of σ 2 α (α = ξ or η) is smallest when ϕ α = ϕ ± π 2, meaning that the basalplane moments appearing just below T N,where
19 86 2. MAGNETIC STRUCTURES this coefficient vanishes, are locked to be out of phase by 90 with the caxis component. This phase difference arises because the transverse MF susceptibility χξξ o for the single sites increases as the caxis exchange field falls. Using the estimate (2.1.21b) forthebtensor, and the hightemperature value for A ξ, we find the transition temperature to be k B T N 1 3 J(J +1)J (Q) [ (J 1 2 )(J )B0 2 /k B T N 3 20 { (J +1) 2 }σ 2 Q ]. (2.1.38) A slightly better estimate may be obtained by calculating the MF value of the transverse susceptibility directly, in the presence of a nonzero exchange field, which just causes the replacement of σ Q in (2.1.38) by 3σ Q J (Q)/[J(J +1)k B T N ] (Miwa and Yosida 1961). However, both results are based on the hightemperature expansion, which ceases to be valid at low temperatures. In the zerotemperature limit, χξξ o of the ith site remains finite, being of the order J/h eff iζ. This saturation implies that the transition does not necessarily occur. If the caxis is favoured too strongly by the anisotropy terms, the basalplane components remain disordered at low temperatures, as is observed in Tm. When the basalplane moments order, as in Er, eqn (2.1.38) may give a reasonable estimate of the transition temperature. As mentioned previously, the modulation of the basalplane moments, just below T N,islockedat90 out of phase with that of the caxis component. Since this applies to both components, only a linearlypolarized moment can develop at the transition temperature, with a relative magnitude σ =(σξ 2 + σ2 η )1/2, in a specified but arbitrary direction in the plane. If the sixthpower terms are included in the free energy, B6 6 favours either the a orthe bdirections, but there are still six equivalent but different directions of the moments in the basal plane with equal energies. To be specific, we may assume that B6 6 is negative and that the ordered moments in the basal plane establish themselves along the ξaxis. In this case, the moments all lie in the ξ ζ plane in an elliptic cycloidal structure. Displaced to a common origin, the hodograph of the moments is an ellipse, with its principal axes along the ξ andζaxes, as is illustrated, in connection with our discussion of Er, in Fig. 2.6 on page 120. The caxis moments will still show a strong tendency towards squaring up with decreasing temperature, as long as they are large compared with the basalplane moments. Because of the phaselocking between the components, the higher oddharmonics in the modulation of the caxis moments will also be reflected in the basalplane. At high temperatures, B2 0 is the dominant anisotropy parameter, and its sign determines whether the system orders in a helically or longitudinally polarized structure, when Q 0 is along the caxis. If B2 0 is still
20 2.1 MEANFIELD THEORY OF MAGNETIC ORDERING 87 the most important axialanisotropy parameter in the lowtemperature limit, the helix is still a stable structure at T = 0 whereas, in the longitudinally polarized case, the tendency to minimize the variation of the lengths of the moments may result in two different paths. Either the system stays in the longitudinally polarized phase, ending up as a (commensurable) squarewave structure at T = 0, or it goes through a transition to an elliptic cycloidal structure. The path which is chosen depends on the magnitude of B2 0 ; if the effective axial anisotropy B2 0 O0 2 is sufficiently large, the ordering of the basalplane moments is quenched. It has already been mentioned in Section 1.5 that this anisotropy depends on the magnetization, being proportional approximately to σ 3. We shall discuss this renormalization in more detail in the next section, but it is worth mentioning here that this behaviour of the effective anisotropyparameter means that there is an intermediate range of B2 0 for which the system makes a transition to the elliptic cycloidal structure, but leaves it again at a lower temperature, by returning to the longitudinally polarized phase when B2 0 O0 2 becomes large enough. When B4 0 and B0 6 are included, a more realistic situation may occur, in which the lowtemperature anisotropy favours an orientation of the moments making an angle θ with the caxis, which is neither 0orπ/2 but some, temperaturedependent, intermediate value. In the case of the helix, this means that there will be a critical temperature T N (below T N ) where the effective axial anisotropy parameter vanishes, andbelowwhichthecaxis moments are ordered. If the ordering wavevector for the caxis component is the same as the helical wavevector, the structure adopted is the tilted helix. However the twoion coupling between the caxis moments, J (q) withq caxis, is not restricted by any symmetry argument to be equal to the coupling between the basalplane moments, J (q) =J (q) withitsmaximumatq = Q 0. If the maximum of J (q) lies at a q Q 0,theccomponent will order at this wavevector and not at Q 0, as the extra energy gained by the ccomponent by locking to the basalplane moments is very small, being proportional to {B6 6 O6 6 /(Jσ)2 J (Q)} 2. When B2 0 is negative, a nonzero value of θ favours the elliptic cycloidal structure, compared to the longitudinally polarized phase. If the system is already in the cycloidal phase, it may undergo a new secondorder transition, in which the plane of the ellipse starts to tilt away from the ξ ζ plane, in close correspondence with the behaviour of the helix. Referring back to eqn (2.1.37), we observe that this transition occurs when the coefficient of ση,withϕ 2 η = ϕ (+π) =ϕ ξ ± π/2, becomes zero. The phaselocking energy, comprising the terms in (2.1.37) involving ϕ η, is more important in this case than in the helix, but it is nevertheless possible that the third component may order at a wavevector different from that of the other
1 OneDimensional Magnetism
1 OneDimensional Magnetism HansJürgen Mikeska 1 and Alexei K. Kolezhuk 1,2 1 Institut für Theoretische Physik, Universität Hannover, Appelstaße 2, 30167 Hannover, Germany, mikeska@itp.unihannover.de
More informationClassical Mechanics. Joel A. Shapiro
Classical Mechanics Joel A. Shapiro April 21, 2003 Copyright C 1994, 1997 by Joel A. Shapiro All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted
More informationSpaceTime Approach to NonRelativistic Quantum Mechanics
R. P. Feynman, Rev. of Mod. Phys., 20, 367 1948 SpaceTime Approach to NonRelativistic Quantum Mechanics R.P. Feynman Cornell University, Ithaca, New York Reprinted in Quantum Electrodynamics, edited
More information11 The Kondo Effect. Frithjof B. Anders Theoretische Physik II Technische Universität Dortmund. Contents
11 The Kondo Effect Frithjof B. Anders Theoretische Physik II Technische Universität Dortmund Contents 1 Introduction 2 1.1 Resistance minimum............................... 3 1.2 Anderson model..................................
More informationBreakdown of Local Thermodynamic Equilibrium...
II Stellar Atmospheres Copyright (2003) George W. Collins, II 15 Breakdown of Local Thermodynamic Equilibrium... Thus far we have made considerable use of the concepts of equilibrium. In the stellar interior,
More informationOrdering, metastability and phase transitions in twodimensional systems
J. Phys. C: Solid State Phys., Vol. 6, 1973. Erinted in Great Britain. @ 1973 Ordering, metastability and phase transitions in twodimensional systems J M Kosterlit7 and D J Thouless Department of Mathematical
More informationOPRE 6201 : 2. Simplex Method
OPRE 6201 : 2. Simplex Method 1 The Graphical Method: An Example Consider the following linear program: Max 4x 1 +3x 2 Subject to: 2x 1 +3x 2 6 (1) 3x 1 +2x 2 3 (2) 2x 2 5 (3) 2x 1 +x 2 4 (4) x 1, x 2
More informationAn Iteration Method for the Solution of the Eigenvalue Problem of Linear Differential and Integral Operators 1
Journal of Research of the National Bureau of Standards Vol. 45, No. 4, October 95 Research Paper 233 An Iteration Method for the Solution of the Eigenvalue Problem of Linear Differential and Integral
More informationOrthogonal Bases and the QR Algorithm
Orthogonal Bases and the QR Algorithm Orthogonal Bases by Peter J Olver University of Minnesota Throughout, we work in the Euclidean vector space V = R n, the space of column vectors with n real entries
More informationTHE PROBLEM OF finding localized energy solutions
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Reweighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,
More informationOBSTACLES ON THE WAY TOWARDS THE QUANTIZATION OF SPACE, TIME AND MATTER and possible resolutions
SPIN2000/20 OBSTACLES ON THE WAY TOWARDS THE QUANTIZATION OF SPACE, TIME AND MATTER and possible resolutions Gerard t Hooft Institute for Theoretical Physics University of Utrecht, Princetonplein 5 3584
More informationSemiSimple Lie Algebras and Their Representations
i SemiSimple Lie Algebras and Their Representations Robert N. Cahn Lawrence Berkeley Laboratory University of California Berkeley, California 1984 THE BENJAMIN/CUMMINGS PUBLISHING COMPANY Advanced Book
More informationBaryon Number Generation in the Early Universe
Baryon Number Generation in the Early Universe 1980 The generation of an excess of baryons over antibaryons in the very early universe due to CPand Bviolating interactions is described. The Boltzmann
More informationTwolevel states in glasses
Rep. Prog. Phys. 50 (1987) 16571708. Printed in the UK Twolevel states in glasses W A Phillips Cavendish Laboratory, University of Cambridge, Madingley Road, Cambridge CB3 OHE, UK Abstract This review
More informationSampling 50 Years After Shannon
Sampling 50 Years After Shannon MICHAEL UNSER, FELLOW, IEEE This paper presents an account of the current state of sampling, 50 years after Shannon s formulation of the sampling theorem. The emphasis is
More informationHighDimensional Image Warping
Chapter 4 HighDimensional Image Warping John Ashburner & Karl J. Friston The Wellcome Dept. of Imaging Neuroscience, 12 Queen Square, London WC1N 3BG, UK. Contents 4.1 Introduction.................................
More informationA Molecular Dynamics Study of Slow Base Flipping in DNA using Conformational Flooding
770 Biophysical Journal Volume 93 August 2007 770 786 A Molecular Dynamics Study of Slow Base Flipping in DNA using Conformational Flooding Benjamin Bouvier and Helmut Grubmüller Theoretical and Computational
More informationWMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation
IEEE TRANSACTIONS ON CONTROL SYSTEMS TECHNOLOGY, VOL. 10, NO. 6, NOVEMBER 2002 835 WMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation Giuseppe Oriolo, Member,
More informationScience, New Series, Vol. 220, No. 4598. (May 13, 1983), pp. 671680.
Optimization by Simulated Annealing S. Kirkpatrick; C. D. Gelatt; M. P. Vecchi Science, New Series, Vol. 220, No. 4598. (May 13, 1983), pp. 671680. Stable URL: http://links.jstor.org/sici?sici=00368075%2819830513%293%3a220%3a4598%3c671%3aobsa%3e2.0.co%3b28
More informationIndexing by Latent Semantic Analysis. Scott Deerwester Graduate Library School University of Chicago Chicago, IL 60637
Indexing by Latent Semantic Analysis Scott Deerwester Graduate Library School University of Chicago Chicago, IL 60637 Susan T. Dumais George W. Furnas Thomas K. Landauer Bell Communications Research 435
More informationPhysik Department. Matrix Product Formalism
Physik Department Matrix Product Formalism Diplomarbeit von María Gracia Eckholt Perotti Angefertigt an der Technische Universität München und am MaxPlanckInstitut für Quantenoptik Garching, September
More informationIEEE TRANSACTIONS ON INFORMATION THEORY, VOL. 52, NO. 4, APRIL 2006 1289. Compressed Sensing. David L. Donoho, Member, IEEE
IEEE TRANSACTIONS ON INFORMATION THEORY, VOL. 52, NO. 4, APRIL 2006 1289 Compressed Sensing David L. Donoho, Member, IEEE Abstract Suppose is an unknown vector in (a digital image or signal); we plan to
More informationThe Pendulum as a Useful Example: ActionAngle Variables and Perturbation Theory
The Pendulum as a Useful Example: ActionAngle Variables and Perturbation Theory. The Simple Pendulum: Setup and Motion in Terms of Action Angle Variables We consider a simple pendulum, of mass m and length
More informationFoundations of Data Science 1
Foundations of Data Science John Hopcroft Ravindran Kannan Version /4/204 These notes are a first draft of a book being written by Hopcroft and Kannan and in many places are incomplete. However, the notes
More informationINTRODUCTION TO THE THEORY OF BLACK HOLES
ITPUU09/11 SPIN09/11 INTRODUCTION TO THE THEORY OF BLACK HOLES internet: Gerard t Hooft Institute for Theoretical Physics Utrecht University and Spinoza Institute Postbox 80.195 3508 TD Utrecht, the
More informationFoundations of Data Science 1
Foundations of Data Science John Hopcroft Ravindran Kannan Version 2/8/204 These notes are a first draft of a book being written by Hopcroft and Kannan and in many places are incomplete. However, the notes
More informationAn Introduction to the NavierStokes InitialBoundary Value Problem
An Introduction to the NavierStokes InitialBoundary Value Problem Giovanni P. Galdi Department of Mechanical Engineering University of Pittsburgh, USA Rechts auf zwei hohen Felsen befinden sich Schlösser,
More informationSymmetryoperations, point groups, space groups and crystal structure
1 Symmetryoperations, point groups, space groups and crystal structure KJ/MV 210 Helmer Fjellvåg, Department of Chemistry, University of Oslo 1994 This compendium replaces chapter 5.3 and 6 in West. Sections
More informationWHICH SCORING RULE MAXIMIZES CONDORCET EFFICIENCY? 1. Introduction
WHICH SCORING RULE MAXIMIZES CONDORCET EFFICIENCY? DAVIDE P. CERVONE, WILLIAM V. GEHRLEIN, AND WILLIAM S. ZWICKER Abstract. Consider an election in which each of the n voters casts a vote consisting of
More informationThe Backpropagation Algorithm
7 The Backpropagation Algorithm 7. Learning as gradient descent We saw in the last chapter that multilayered networks are capable of computing a wider range of Boolean functions than networks with a single
More information